Transcript of "Gallium nitride ga n led crystal growing techniques report"
Introduction to Gallium Nitride LED Tsinghua University, Beijing China Department of Electronics EngineeringReport on: Introduction to GaN LED’s Tayyab Farooq (阿里) 2012280158 1
Introduction to Gallium Nitride LEDContentsContents...........................................................................................................................................2Abstract: This report defines the introduction of Gallium Nitride and its uses in Opto- Industry. The discovery of Gallium Nitride in Photo-Electronics industry is little bit latest as compare to other light sourcing materials. So now a days, there are a lot of research doing on GaN based LED’s. Recently GaN and its alloys have an interesting application due to their direct and wide band gap energy. The growth and successful doping of high quality GaN single crystal have led to optoelectronic devices from blue to near UV region, as well as devices for high power and high temperature electronics. The aim of this paper is to review the different growth techniques used for GaN epitaxial growth, including HVPE, MOCVD, MBE and their recent modifications. 2
Introduction to Gallium Nitride LED In this report, I try to put my focus on techniques used for GaN crystal growth. First I discuss about Gallium Nitride, and its physical and chemical behaviour, then I highlight its substrates, and at the end I focus on GaN crystal Growth Techniques.IntroductionIn 1879 Thomas Alva Edison invented the incandescent lamp. This invention has been abreakthrough in human progress since it permitted people not to be strictly tied up to sunriseand sunset. The success of this device is due to its simplicity and to the quality of the lightproduced, very similar to sunlight. Unfortunately, incandescent lamps have a very low eﬃciency,95 % of the absorbed power is dissipated in heat, and also their average lifetime is very short, justover 1000 hours.Later technologies regard the ﬂuorescent lamp. These lamps are capable of higher eﬃciencies(approximately of 25 %) and of a longer lifetime (approximately of 10000 hours) compared toincandescent lamps. Furthermore, their characteristics make their ratio quality/price moreconvenient. The main drawback of these lamps compared to incandescent lamps is that the whitelight they emit is perceived by the human eye as “colder”.In the last few years research on illumination devices has focused on semiconductor-based solidstate devices, and particularly Light-Emitting Diodes (LEDs).The year that marks the beginning of illumination through semiconductors is 1907, when H. J.Round noticed that a sample of silicon carbide emitted a weak yellow light when exposed to avoltage of 10 V. This ﬁrst experience was completely random and only in 1950’s research startedwith some know- ledge. Research gave good results: in 1962 the ﬁrst red LED was built in AsGaPby N. Holonyak from General Electric. This LED had a luminous eﬃciency of 0.1 lm/W. He had theidea to take a diode in GaAs and expand its bandgap with some phosphor to have emission in the 3
Introduction to Gallium Nitride LEDvisible range of the electromagnetic spectrum. Research continued on compoundsemiconductors of groups III-V and II-VI. Soon it had been possible to cover most of the visiblespectrum, but only with indicator LEDs (for red and IR-LEDs the material used was AlGaAs, forgreen LEDs the materials used were GaP and GaP: N). in the 1950’s construction techniquesimproved, so it started to be possible to produce high eﬃciency LEDs. In 1995 S. Nakamuraproduced the ﬁrst blue LED in InGaN/GaN. The following step has been to produce high eﬃciencyLEDs emitting white light.The main advantage of today LEDs is their high eﬃciency, which can be even very near to 100 %.Since the 21 % of the world’s electrical energy is used for illumination, replacing even only half ofthe light sources with LEDs we would have a global saving of electricity of more than 10 %. Thatwould involve substantial economic beneﬁts, but also a signiﬁcant reducing of the environmentalpollution.Research on LEDs is giving always better results, thus LEDs are considered the main investment inthe lighting ﬁeld for the future.Besides their high eﬃciency LEDs have also got many other advantages such as:• A minimum production of heat compared to traditional illumination devices• an average lifetime of 100000 hours, which is 100 times longer than that one of anincandescent lamp, and 10 times longer than that one of a ﬂuorescent lamp• The capability to generate light of any colour and with a much accentuated selectivity• They are very small• They are very strong and resistantHowever LEDs have also disadvantages such as:• the lack of compatibility of the lattice constants and the thermal co-efﬁcient of Gallium Nitridewith those of the materials used to produce substrates and charge conﬁnement layers, which canlead to the generation of crystal defects• A technology growth which is not yet reﬁned and reliable• Gallium Nitride grows unintentionally N-doped, the unintentional N-doping makes diﬃcult tocreate P-doped layers• The diﬃcult realization of Ohmic contacts• The presence of the piezoelectric eﬀect, which reduces the eﬃciency of the active zone• The generation of deep levels in the energy gap that can reduce the eﬃciency of radiaterecombination and vary the ﬁxed charge distribution 4
Introduction to Gallium Nitride LEDNowadays LEDs have got many applications, among which we can mention the following:• Large displays for stadiums, airports, stations and dynamic decorative displays• Traﬃc lights, emergency exits, emergency lights and brake and position lights on vehicles• Billboards• Illumination with white LEDs• Architectural decorations for buildings• Backlight of LCD TVGallium Nitride Gallium Nitride is a binary group III/group V direct bandgap semiconductor material. Since thegrowth and doping problems have been resolved it has become the most widely usedsemiconductor for optoelectronic devices. In optoelectronic devices, in fact the arrival of GaN hasbeen necessary in order to develop blue and green light emitting diodes and Deep UltravioletLEDs. Gallium Nitride is a very hard and mechanically stable material and has a large heatcapacity.Gallium Nitride chemical and physical propertiesGallium Nitride, thanks to its chemical and physical properties, is, together with GaAs, one of themost attractive and used semiconductor materials for producing electronic and especiallyoptoelectronics devices. Gallium Nitride can crystallize both in the wurtzite and the zincblend structure. As far ascrystallography is concerned the two diﬀerent structures present many analogies, but they arestrongly diﬀerent form the electrical and doping point of view. Wurtzite crystalline structure ischaracterized by a lattice which has a hexagonal structure with equal constants a and b. The caxis is orthogonal to the hexagonal plane. The lattice is in fact a sequence of Gallium and Nitrideatom surfaces which are placed along c axis. Thus, the wurtzite crystallographic structure ischaracterized by two hexagonal lattice structures compenetrated. Zincblend lattice is formedwith Nitride atoms which are placed in a cubic structure and bonded to a thetraedric structureformed by Gallium atoms. Thus, the zincblend lattice is formed by two cubic lattice structurescompenetrated.The deﬁnition of the crystalline structure of GaN is given by three lattice constants (a, b, c) andthree angles α, β and γ. Wurtzite has constants a = b = c, α = β = 90°, γ = 120°, instead zincblendhas constants a = b = c and α = β = γ = 90° typical of a cubic structure. The two crystallinestructures are shown in Figs. 1.1 and 1.2. 5
Introduction to Gallium Nitride LEDFigure 1.1: Wurtzite crystalline structure Figure 1.2: Zincblend crystalline structureGALLIUM NITRIDE CHEMICAL AND PHYSICAL PROPERTIESThe lattice constants of the crystal have a strong relation with the electrical properties of thesemiconductor. For example smaller is the lattice structure, greater is the energy gap. Thisphenomenon coincides also with the relation between temperature and energy gap, in fact ahigher temperature produces a widening of the crystal structure, and thus a lower energy gap.Fig. 1.3 presents diﬀerences between wurtzite GaN, zincblend GaN and other semiconductors. 6
Introduction to Gallium Nitride LED Figure 1.3: Semiconductor parameter comparison Gallium Nitride crystal has a light probability of dislocations and lattice defect formation due tothe strong bonding energy between the GaN atoms. For this reason GaN is very stable and usedfor high power applications.The use of GaN in the optoelectronic ﬁeld is basically related to its electronic band structure,which has a direct energy gap. The electronic band structure of Wurtzite GaN is presented in Fig.1.4. 7
Introduction to Gallium Nitride LED Figure 1.4: Wurtzite GaNDiﬀerently from other composite semiconductors, Gallium Nitride has a sensible degeneration ofthe valence band. This phenomenon is related to the high electric ﬁeld due to the crystallinestructure. Thus wurtzite GaN may be considered as an intrinsic deformation structure, and so,less inﬂuence able by external deformation forces. In optoelectronic applications the mostimportant transition is the fundamental one, from the maximum of the valence band to theminimum of the conduction band. The energy related to this transition is 3.504 eV, correspondingto a wavelength of 355 nm in void. The wide energy gap and good thermal stability of GaN is alsoadvantageous for high-temperature (HT) and high power electronics. Gallium Nitride forms solid solutions with AlN and InN, making a wide range (1.9 - 6.2 eV) ofenergy gap possible. This ability to form alloys is essential for producing speciﬁc wavelengths forLEDs. Alloys are also very useful in creating hetero junctions with potential barriers into thedevice structures.Heat dissipation in GaN-based devices is facilitated by GaN’s high thermal conductivity comparedto that one of silicon and Gallium arsenide. Both n and p -type conductivities are possible in GaN.Brief history of GaN technologyThe ﬁrst growth of GaN is attributed to Johnson, who describes how to obtain Gallium Nitridewith a chemical reaction involving Gallium and ammonia:2Ga + 2 NH3 2GaN + 3H2Later on, in 1969, the ﬁrst quite eﬃcient epitaxial growth technique is settled up by Maruska andTietjen. From metallic Gallium and chloridric acid, they established a reaction between Galliumand ammonia: 8
Introduction to Gallium Nitride LEDGaCl + NH3 GaN + HCl + H2This technique grants a high growing rate, so thick layers of GaN could be obtained with theadvantage of a little lattice mismatch from the bulk. Unfortunately electrical characteristics ofdevices grown with Maruska and Tietjen techniques are very poor.Substrates Gallium Nitride, unlike other semiconductors, needs a substrate to grow on. Gallium Nitridedevices are generally created with a thin GaN ﬁlm deposited on a diﬀerent substrate (a materialwhich is not GaN); that is a hetero-epitaxial thin ﬁlm. As a consequence of hetero-epitaxy, thequality of the GaN ﬁlm is very dependent on the properties of the substrate. In order to grow aGaN crystal virtually free of dislocations and defects, the two materials must have latticeconstants and thermal expansion coeﬃcients as close as possible. Defects such as threadingdislocations, inversion domains, and the un-intentional incorporation of impurities into theepitaxial GaN layer resulting from hetero-epitaxy are strongly dependent with the type ofsubstrate used. Finding a substrate with these characteristics has been a real youth problem.There are priory few materials that match the characteristics needed for producing good qualityGaN ﬁlms: • Sapphire • Silicon carbide • Silicon • Gallium NitrideSapphireSingle crystal sapphire, i.e. single crystal di-aluminium trioxide, Al 2O3, was the original substrateused in Maruska and Tietjen’s pioneering studies of GaN epitaxy by hydride vapour phase epitaxy(HOPE) in 1969, and it remains the most commonly employed substrate for GaN epitaxy. Thelarge lattice constant mismatch (∼ 15 %) between sapphire (Al2O3) and GaN leads to highdislocation density (1010 cm2) in the GaN epitaxial ﬁlm. This high defect density in the GaNepitaxial ﬁlm reduces the charge carrier mobility, the minority carrier lifetime, and decreases thethermal conductivity, all of which degrade performances of devices made of GaN. Sapphire’scoeﬃcient of thermal expansion is greater than GaN’s one. This produces biaxial compressivestress in the GaN layer as it cools down from the deposition temperature. Fig. 1.5 shows GaN onsapphire. 9
Introduction to Gallium Nitride LED Figure 1.5: GaN on sapphire crystal structure and lattice mismatchOne of the reasons why sapphire has been as successful as a substrate for GaN epitaxy is simplythat much more research has gone into developing procedures for producing good quality GaNﬁlms on it compared to other substrates.The large lattice constant mismatch between sapphire and GaN causes the GaN ﬁlm to becompletely relaxed (not strained) essentially from the beginning of growth. Consequently, thedefect density at the sapphire substrate/GaN ﬁlm interface is very high.Fig. 1.6 shows GaN defects and dislocations on sapphire substrate with buﬀer layer. Figure 1.6: GaN defects and dislocations on sapphire substrate with buﬀer layerThe detrimental eﬀect of the large lattice constant mismatch between sapphire and GaN must beimproved by a sophisticated processing scheme. 10
Introduction to Gallium Nitride LED1. The sapphire substrate surface is treated to remove contaminants, remnant polishingdamages, and to produce a step and terrace surface structure2. The sapphire substrate is nitrated to alter the wetting characteristics of the deposited layer3. A thin buﬀer layer of either GaN or AlN (usually 10 - 100 nm thick) is deposited at a lowtemperature and annealed to produce a surface ready for the ﬁnal epitaxial growth. Theadvantage of sapphire for optoelectronic devices consists in its transparency to visible light.Unfortunately sapphire is an electrical insulator, thus, all devices electrical contacts must bemade on the front side of the devices, reducing the available area for devices and complicatingdevices fabrication. An example of a LED with a sapphire substrate is presented in Fig. 1.7. Figure 1.7: Example of a LED with a sapphire substrateThe main characteristic is that both contacts have to be placed on the same surface, obviouslyreducing the emitted light ﬂux. This drawback can be minimized with ﬂip-chip mounting, aparticular technique consisting in mounting the device reversed with light ﬂowing out from thesubstrate. The processing of a ﬂip chip mounting is similar to conventional IC fabrication with theaddition of a few steps. Near the end of the process, the attachment pads are “metalized” tomake them more suitable for being soldered onto. A small dot of solder is then deposited oneach of the pads. The chips are then cut out of the wafer as normal. No additional processing isrequired, and there is no mechanical carrier at all. To attach the ﬂip chip into a circuit, it isinverted to bring the solder dots down onto connectors on the underlying electronics or circuitboard. The solder is then re-melted to produce an electrical connection, typically using anultrasonic process. 11
Introduction to Gallium Nitride LEDSilicon carbideSingle crystal silicon carbide (6H-SiC) is another substrate available for GaN epitaxy. The twomaterials have a reduced lattice constant mismatch, about 3.5 %, so due to this reducedmismatch, a good quality GaN ﬁlm can be grown on a SiC substrate. Consequently, the defectdensity at the SiC substrate/GaN ﬁlm interface is lower than one at the sapphire substrate/GaNﬁlm. Conductive SiC substrates are available, making electrical contacts to the backside of the SiCsubstrate possible, therefore simplifying the device structure compared to sapphire substrates.However, SiC does have its disadvantages. Gallium Nitride epitaxy directly on SiC is problematic,due to poor wetting between these materials. This can be remedied by using an AlN or Alx Ga1−xN buﬀer layer, but such layers increase the resistance between the SiC substrate and the GaNﬁlm. Even though the lattice constant mismatch between SiC and GaN is smaller than that onebetween sapphire and GaN, it is still suﬃciently large to cause a large density of defects to formin the GaN layer. Preparing smooth silicon carbide surfaces is diﬃcult, thus, its surface roughnessis an order of magnitude (1nm RMS) higher than that one of sapphire (0.1nm RMS). Thisroughness and also remnant subsurface polishing damages are sources of defects in the GaNepitaxial layer. The dislocation density in SiC goes from 103 to 104 cm2, and these defects maypropagate into the GaN epitaxial layer and degrade devices performances. Silicon carbide’sthermal expansion coeﬃcient is less than that one of AlN or GaN, thus, the epitaxial grown ﬁlmsare typically under biaxial tension at room temperature. Last, the cost of silicon carbidesubstrates is high, and currently single crystal SiC is produced by relatively few manufacturers.Gallium NitrideThe best substrate for GaN epitaxy is of course Gallium Nitride itself. The use of GaN as thesubstrate for GaN epitaxy, that is homo-epitaxy, eliminates all the problem of hetero-epitaxy, butonly in the last few years it has been possible to grow epitaxial GaN on a GaN substrate. Homo-epitaxy oﬀers better control compared to hetero-epitaxy over the crystal polarity and strainedlayer thickness. Gallium Nitride homo-epitaxy of smooth ﬁlms does not require nitration orbuﬀer layers, as required instead for GaN hetero-epitaxy, for example with sapphire and siliconcarbide.Although there are several techniques under development for producing single crystal GaN bulksincluding growth by vapour phase transport, growth from supercritical ﬂuids, and growth fromsodium ﬂuxes, only high pressure growth from solutions and hydride vapour phase epitaxy haveproduced large area crystals. The production of a thick GaN bulk layer is generally obtained withHVPE (Hydrogen Vapour Phase Epitaxy) over a layer of sapphire, and then the GaN layer isremoved and used for homo-epitaxy. This kind of growth is quite fast and for a thick GaN layerthe dislocation density at the surface is small. Up to this date GaN optoelectronic devices built ona GaN substrate are entering the market solving critical problems of eﬃciency, maximum outputpower and stability. 12
Introduction to Gallium Nitride LEDGaN GrowthFabrication of high-brightness LEDs involves the growth of multilayer semi- conductor ﬁlms overappropriate substrates. Then the wafers are diced, the chips are equipped with contacts, and theLEDs are encapsulated into transparent plastic domes or other types of packages. Developmentof hetero-structure/epitaxy growth techniques has required many eﬀorts by semiconductorphysicists and materials engineers. These techniques must facilitate precise and reproduciblecontrol of the composition and thickness of the grown layers. Also, the growth methods used inmass production must be cost-eﬃcient.Epitaxial Growth TechniquesThe main epitaxial GaN growth techniques are the following:• HVPE (Hydrogen Vapour Phase Epitaxy)• MBE (Molecular Beam Epitaxy)• MOCVD (Metal-Organic Chemical Vapour Deposition)• MEMOCVD (Migration Enhanced Metal-Organic Chemical Vapour Deposition)• ELO (Epitaxial Lateral Overgrowth)HVPE (Hydrogen Vapour Phase Epitaxy)This technique is based on the reaction between ammonia (NH3) as a source of Nitrogen andvapour Gallium Chloride (GaCl) as a Gallium source to obtain Gallium Nitride. The reaction isperformed in a Hydrogen or Nitrogen rich ambient:GaCl (g) + NH3 (g) GaN(s) + HCl (g) + H2 (g)The HVPE growth rate is quite high (30 - 130 µm/h), but the GaN obtained with this technique hasthe drawback to be rich of dislocation and lattice defect. For this reason HVPE is now only used tobuild thick layers of GaN on sapphire, GaN layers used as a bulk substrate for GaN homoepitaxy. 13
Introduction to Gallium Nitride LEDMBE (Molecular Beam Epitaxy)This technique is an Ultra-High-Vacuum (UHV) technique based on a simple reaction and it hasbeen used, since 1958, for Nitride, II-VI compounds and silicon growth. MBE is performed atlower temperature than HVPE.In the last few years, it has been possible to use N 2 as a source of Nitrogen by means of a plasmasource (PMBE, Plasma-Assisted MBE). This could not be done in the past decades due to N 2strong bonding energy so the source of N was ammonia (NH 3), but this had the strong drawbackto be Hydrogen rich. Fig. 1.8 shows the structure of a PMBE reactor. The reaction chamberconditions, a constant pressure of 10−10 torr, and a lower temperature than HVPE permit the useof volatile elements like indium and Magnesium. The Gallium atoms are extracted with thermalevaporation from eﬀusion cells connected to the main chamber and regulated with a shutter.During operation, RHEED (Reﬂection High Energy Electron Diﬀraction) is often used formonitoring the growth of the crystal layer. Controlling shutters in front of each eﬀusion cell,allow precise control of the thickness of each layer, down to a single layer of atoms. Intricatelayers of diﬀerent materials may be fabricated this way allowing the building up of hetero-structures and MAW structures. Figure 1.8: Structure of a PMBE reactor with RHEED gunMOCVD (Metal-Organic Chemical Vapour Deposition)Metal-Organic Chemical Vapour Deposition is the most used process for producing epitaxial ﬁlmsfor optoelectronic devices and has been ﬁrst studied in 1990. Vapour phase group III elementsand group V elements react in an MOCVD chamber at atmospheric pressure over a heated 14
Introduction to Gallium Nitride LEDsubstrate. The technique consists of transport of vapour source materials, i.e. pre- cursors,subsequent reaction of these source materials in the heated zone, and deposition of the ﬁnalcrystalline product on a substrate. Precursors of group III elements are metal-organiccompounds, either tri-methyl or tri-ethyl based. The most extensively used precursors of group IIIelements are tri- methyl-aluminium Al (CH 3 )2 (TMAl), tri-methyl- Gallium Ga (CH3)2 (TMGa), andtri-methyl-indium In (CH3)2 (TMln) respectively for aluminium, indium and Gallium growth.Precursors of group V elements are the hydrides phosphine (PH 3) and ammonia (NH3) respectivelyfor phosphide and Nitride growth. Typical dopant precursors are the metal-organic compoundsdi- ethyl-zinc (DEZn), di-methyl-zinc (DMZn), magnesium (Cp2Mg), and di-ethyl-tellurium (DETe),as well as hydrides: silane (SiH4) and di-silane (Si2 H6). Although reactions involved in MOCVDcontain intermediate stages which are not completely understood, by MOCVD high qualityepitaxial layers are obtained. Fig. 1.9 shows the structure of a MOCVD reactor. Figure 1.9: Structure and elements of a MOCVD reactor 15
At the beginning of the growth process the substrate is placed over a rotating graphite plateinitially at 1150 °C, then temperature is lowered to 450 °C allowing the building up of a lowtemporary buﬀer layer, then for the real GaN growth the temperature is raised to approximately1075 °C.To increase the eﬃciency of the process, Nakamura in 1997 has developed a new system ofMOCVD with the aim to increase the rate of metal-organic compounds that reach the heatedsubstrate and perform a complete reaction. In Nakamura’s system, also called two ﬂow MOCVD,a gas ﬂows parallel and another one ﬂows perpendicular to the surface. The precursors aredelivered by the horizontal ﬂow through a quartz nozzle, ﬂowing parallel to the substrate. Thevertical ﬂow transports inactive gases (N 2 + H2) and is needed to bring the precursors into contactwith the substrate. This conﬁguration suppresses thermal convection currents on the substrateand cools the reactant gases just before they react. This lower temperature leads to more stablereactions and higher-quality grown ﬁlms. A typical growth rate is 4 µm/h. Growth takes place atatmospheric or lower pressure. With TF-MOCVD it’s possible to achieve a high speed growth withan acceptable dislocation density at the surface of the grown layer. With this technique it ispossible to obtain GaN and several type of GaN alloys with enough accuracy to realize layers withthe desired energy gaps. A problem is still present with InGaN alloy with high indium levels:Indium fragmentation occurs and thin layers present a heterogeneous structure. The highhydrogen level during reactions is the weak point of the process and several studies haveaccused hydrogen to be the principal responsible for GaN degradation phenomena.MEMOCVD (Migration Enhanced Metal-Organic Chemical Vapour Deposition)The technique Migration Enhanced Metal-Organic Chemical Vapour Deposition (MEMOCVD) hasbeen developed by SETI (Sensor Electronic Techno- logy Inc.). MEMOCVD is an epitaxialtechnique for growing AlN/GaN/InN epitaxial ﬁlms and hetero-structure layers using PrecursorsControlled pulsed ﬂow to achieve accurate control of the thickness of the grown ﬁlms over largearea substrates. It grants for example lower temperature than MOCVD. Tri- methyl Aluminium(TMAl), Trimethyl Gallium (TMGa), Tri-methyl Indium (TMIn) and ammonia (NH3) are used asprecursors of Al, Ga, In and N, respectively. MEMOCVD is an improved version of Pulsed AtomicLayer Epitaxy (PALE), which deposits quaternary Alx Iny Ga1−x−y N layers by repeats of a unit cellgrown by sequential (metal-organic) pulses of Al, In, Ga precursors and of NH3 While in PALE theduration of each pulse is ﬁxed, and the NH3 pulse always follows each (metal-organic) pulse, theduration of precursor pulses in MEMOCVD are optimized, and pulses might overlap.This technique bridges the gap between Molecular Beam Epitaxy (MBE) and Metal-OrganicChemical Vapour Deposition (MOCVD). MEMOCVD combines a fairly high growth rate withreduced growth temperature (by more than 150 °C compared to MOCVD) and improved qualityfor grown layers.ELO (Epitaxial Lateral Overgrowth)Epitaxial Lateral Overgrowth (ELO) is a technique consisting in growing GaN on a GaN bulksubstrate generally obtained with HVPE on an initial sacriﬁcial sapphire substrate. The sapphiresubstrate is then removed by means of laser-induced lift oﬀ (LLO), or thermal delamination dueto thermal strain of the interface. Both are damage-free separation techniques of GaN fromsapphire. Overgrowth starts from a GaN seed and proceeds laterally generating a structure called
wing. Several GaN seeds are present so that two wings starting from two adjacent seeds willmeet in a coalescence boundary as presented in Fig. 1.10. Figure 1.10: Schematic illustration of ELO GaN layers sectionA technique of ELO GaN growth is now presented. A 2µm-thick GaN layer is grown on a sapphiresubstrate, after which silicon dioxide (SiO 2) is deposited and patterned, forming stripe masks. TheGaN region is then etched out by reactive ion etching (RIE) and the SiO2 mask is subsequentlyremoved by wet etching. Gallium Nitride is then laterally overgrown using the rectangular GaNstripes as seed regions. A schematic illustration of the cross section of the ELO growth is shown inFig. 1.11. Dislocations and defects are present both in the seed and the coalescence regions.Notice that most of the defects start from the GaN-sapphire interface and have a verticalpropagation direction. Wing regions are instead clear of dislocations. Since dislocations act asnon-radiative centres, reducing the dislocation density is also very eﬀective in increasingeﬃciency of devices.ComparisonTHE Comparison of all the above techniques described is given below.
Table showing the comparison between different epitaxial techniques.ConclusionsNative bulk GaN substrates have been intensively developed by several growth techniques.Availability of this material is constantly increasing in amount, size, doping, and orientationalternatives. Their use in device growth is proven as beneficial for improvement of theperformance of all devices under consideration and for device production cost reduction forsome devices. Further improvement of the substrate quality, along with increasing size anddecreasing cost, is expected in the near future, which will in turn influence the device quality andcost.AcknowledgmentI am very much thankful for my dear teacher, who give me hope, courage and support to learnand work on QUANTUM ELECTRONICS. I am also thankful for her assistant who help me totranslate the problems regarding to my studies to write this report. At last, I must not forget tothanks my FRIEND (WANG XU), he help me to solve my all problems that I face during period.